# Full-Hard (H04) C75700 Nickel Silver

H04 C75700 nickel silver is C75700 nickel silver in the H04 (full hard) temper. The graph bars on the material properties cards below compare H04 C75700 nickel silver to: wrought copper-nickels (top), all copper alloys (middle), and the entire database (bottom). A full bar means this is the highest value in the relevant set. A half-full bar means it's 50% of the highest, and so on.

## Mechanical Properties

Elastic (Young's, Tensile) Modulus

120 *GPa* 17 *x 10 ^{6} psi*

Elongation at Break

3.2 *%*

Poisson's Ratio

0.32

Shear Modulus

45 *GPa* 6.5 *x 10 ^{6} psi*

Shear Strength

350 *MPa* 51 *x 10 ^{3} psi*

Tensile Strength: Ultimate (UTS)

610 *MPa* 88 *x 10 ^{3} psi*

Tensile Strength: Yield (Proof)

580 *MPa* 84 *x 10 ^{3} psi*

## Thermal Properties

Latent Heat of Fusion

200 *J/g*

Maximum Temperature: Mechanical

180 *°C* 350 *°F*

Melting Completion (Liquidus)

1040 *°C* 1900 *°F*

Melting Onset (Solidus)

990 *°C* 1810 *°F*

Specific Heat Capacity

390 *J/kg-K* 0.094 *BTU/lb-°F*

Thermal Conductivity

40 *W/m-K* 23 *BTU/h-ft-°F*

Thermal Expansion

16 *µm/m-K*

## Electrical Properties

Electrical Conductivity: Equal Volume

8.0 *% IACS*

Electrical Conductivity: Equal Weight (Specific)

8.6 *% IACS*

## Otherwise Unclassified Properties

Base Metal Price

30 *% relative*

Density

8.4 *g/cm ^{3}* 520

*lb/ft*

^{3}Embodied Carbon

3.6 *kg CO _{2}/kg material*

Embodied Energy

56 *MJ/kg* 24 *x 10 ^{3} BTU/lb*

Embodied Water

310 *L/kg* 37 *gal/lb*

## Common Calculations

Resilience: Ultimate (Unit Rupture Work)

19 *MJ/m ^{3}*

Resilience: Unit (Modulus of Resilience)

1410 *kJ/m ^{3}*

Stiffness to Weight: Axial

7.8 *points*

Stiffness to Weight: Bending

19 *points*

Strength to Weight: Axial

20 *points*

Strength to Weight: Bending

19 *points*

Thermal Diffusivity

12 *mm ^{2}/s*

Thermal Shock Resistance

23 *points*

## Alloy Composition

Cu | 63.5 to 66.5 | |

Zn | 19.2 to 25.5 | |

Ni | 11 to 13 | |

Mn | 0 to 0.5 | |

Fe | 0 to 0.25 | |

Pb | 0 to 0.050 | |

res. | 0 to 0.5 |

All values are % weight. Ranges represent what is permitted under applicable standards.

## Followup Questions

## Further Reading

ASTM B151: Standard Specification for Copper-Nickel-Zinc Alloy (Nickel Silver) and Copper-Nickel Rod and Bar

ASM Specialty Handbook: Copper and Copper Alloys, J. R. Davis (editor), 2001